Preparation and characterization of Keggin-type heteropolysalts, CoxPMo12O40 (x=0-1.5) Mazari Tassadit1,2, Cadot Emmanuel3, Rabia Chérifa1 1 Laboratoire de Chimie du Gaz Naturel, Faculté de Chimie, USTHB, BP32, El-Alia, 16111Bab-Ezzouar, Alger, Algérie. 2 Département de Chimie, Faculté des Sciences, Université Mouloud Mammeri, Tizi-Ouzou. 3 ILV-UMR 8180 CNRS, Université de Versailles -St Quentin-en-Yvelines, Bâtiment Lavoisier, 45 avenue des Etats-Unis, 78035 Versailles Cedex, France Email: [email protected] Keywords: Polyoxometalates, Cobalt salts, Characterization 1. Introduction: Polyoxometalates (POMs), based transition-metal oxide clusters, have received much attention in various fields such as catalysis, photochemistry, nonlinear optics, biology and medicine1. Their physico-chemical, acidic and oxidative properties can be adjusted according with the nature of constituent elements2. In the field of catalysis, the most studied POMs are those with the Keggin. They were tested in wide variety of reactions in homogeneous and heterogeneous phases. In the redox processes, the nature of counter- cation in the [PMo12O40]3- system can play a significant role. Thus, it has been shown that using Fe(III), vanadyl(VO2+), antimony (Sb3+) or cobalt (Co2+) ionas counter-cation develop of a more favourable distribution of both reduced Mo(V) and oxidized Mo(VI) sites2,3,6. In the present work we report the synthesis and characterization using several techniques of Keggintype heteropolysalts of composition H32xCoxPMo12O40(x=0-1.5) denoted as CoxPMo12. 2. Experimental 2.1. Materials: CoxPMo12 was synthesized by a cation exchange carried out in two stages: in the first step BaxPMo12O40 was prepared from addition of Ba(OH)2 at an aqueous solution of H3PMo12O40 in stoichiometric ratios, and in the second step BaSO4 precipitates after addition of cobalt sulphate. After filtration, the solution was drained to 50°C. CoxPMo12 salts were conserved with any washing. temperature with a Siemens D5000 diffractometer using Cu-Kα radiation(λ=1.5418°A).Thermal analysis (TG) were carried out using a Perkin Elmer Stimiltanous Thermal analyzer STA 6000 and the studies of the morphology of salts using JEOL JSM5800LV Scanning MicroscopIe (SEM). 3. Results 3.1. ATR spectroscopy: The IR vibration wave numbers solids are summarized in Table1. In the low wave number region (1100−500cm−1), the characteristic bands of the Keggin structure were obtained. According to Rocchiccioli-Deltcheff et al4, the bands at 1065, 962, 865, 793 and 561 cm−1 correspond to υas(P–Oa), υas(Mo–Od), υas(Mo–Ob– Mo), υas(Mo–Oc–Mo) and υ(P–O) vibrations, respectively. In Keggin type unit(Fig.1), Oa refers to oxygen atom common to PO4 tetrahedron and one trimetallic group Mo3O13; Ob connects two trimetallicgroups, Oc binds two octahedral MoO6 inside a trimetallic group and Od is the terminal oxygen atom. The whole structure has Td symmetry and corresponds to α isomer. This suggests that primary structure remains intact after the partial and /or the total protons substitution. 2.2. Characterization: Infrared spectroscopy of the solids was recorded on an ATR Thermo scientific Nicolet apparatus. Solution 31P NMR spectra were recorded on a Bruker AC300 apparatus at 121.5MHz. Chemical shifts are referenced to 85% H3PO4. X- ray diffraction (XRD) patterns were recorded at room Figure 1: Structure of Keggin unit Table 1: IR vibration wave numbers (cm–1) of the polyoxometalate CoxPMo12 γPOa γM=Od γMObM γMOcM X=0 1060 962 870 785 X=0,25 1062 964 875 787 X=0,5 1062 966 876 791 X=0,75 1060 964 876 791 X=1 1060 962 874 791 X=1,25 1062 964 877 791 X=1,5 1060 962 876 791 of wavelengths 200–450 nm was observed associated to ligand–metal charge transfers from oxygen to Mo(VI) in the Keggin anion2,5,6. In addition to this broad absorption band, another large charge transfers band was observed above 500-600nm that may be attributed to the d–d transition band of d1 Mo(V) species in octahedral coordination6. This result suggested a partial reduction of Mo (VI) to Mo(V) corresponding to the electron exchange occurring between Co(II) and Mo(VI) as follows: CoII + MoVI CoIII + MoV 3.2. XRD analysis: The X-ray diffractograms of CoxPMo12 are similar to that of the parent acid H3PMo12O40 (Fig. 2), that crystallizes in the triclinic system. These results agree with those of IR spectroscopy show that the ions occupy the counterion position in the polyoxometallate. Figure 3: UV–Visible spectra of Co1.5PMo12 3.6. SEM analysis: From electron microscopy Figure2: XRD patterns of fresh solids 3.3. 31 measurement, H3PMo12 and Co1.5PMo12 show different morphologies as a consequence of the substitution of protons by the Co2+ ions (Fig.4). P NMR: Solution 31P NMR spectrum of CoxPMo12 exhibit only one peak at around -3.18, 3.27,-3.36,-3.4,-3.31,-3.31 and -3.50ppm for x=01.5 respectively. These results evidenced the purity of the heteropolysalts and also show that the chemical shift of 31P is very sensitive to the value of x. Figure 4: SEM images of H3PMo12 and Co1.5PMo12 3.4. Thermal analysis (TG): The TG curves of all salts show tow steps of weight loss. Before 200°C, the weight loss was attributed to crystallization water desorption and between 200– 250°C, water desorption. The latter weight loss allows to calculate the number of protons and therefore to deduce the value of x. Deduced formula for cobalt salts were in good agreement with the theoretical ones (Table 2). Table2: Comparative salts formula Theoretical formula TG deduced formula H3.0Co0PMo12O40 H3.0Co0.0PMo12O40 H2.5Co0.25PMo12O40 H2.53Co0.23PMo12O40 H2Co0.5PMo12O40 H1.96Co0.52PMo12O40 H1.5Co0.75PMo12O40 H1.57Co0.71PMo12O40 H1.0Co1.0PMo12O40 H0.94Co1.03PMo12O40 H0.75Co1.25PMo12O40 H0.6Co1.2PMo12O40 H0.0Co1.5PMo12O40 H0.0Co1.5PMo12O40 3.5 UV–Visible: In the UV–Vis spectra of Co1.5PMo12 salt, (Fig. 3), a large band in the domain Conclusion: The results showed that the gradual cationic exchange method allows to obtain a series of compounds, H3-2xCoxPMo12O40 (x=0-1.5), whose properties could be adjusted according to the value of x. References: SM.Wang, Y. Yuan and Q S.Wang, Journal of Mol Str, 994, 82–86(2011). T.Mazari, C.Marchal-Roch, S. Hocine, N. Salhi and C.Rabia, Journal of Natur Gas Chem , 18:319 (2009).  M. Langpape, J M M.Millet. Appl Catal A, 200:89 (2000).  C. Rocchiccioli-Deltcheff, M .Fournier, R .Frank and R.Thouvenot ,Inorg Chem, 22: 207(1983). J. M. Oliver, J. M. Lopez Nieto, P. Botella and A. Mifsud, Appl Catal. 257: 67 (2004). L. Dermeche , R. Thouvenot , S. Hocine and C.Rabia, Inorganica Chimica Acta 362, 3896–3900 (2009).